|Year : 2018 | Volume
| Issue : 4 | Page : 525-530
Fracture resistance force of primary molar crowns milled from polymeric computer-aided design/computer-assisted manufactured resin blocks
A Mete, Y Yilmaz, SS Derelioglu
Department of Pediatric Dentistry, Faculty of Dentistry, Ataturk University, Erzurum, Turkiye
|Date of Acceptance||11-Sep-2017|
|Date of Web Publication||02-Apr-2018|
Dr. S S Derelioglu
Department of Pediatric Dentistry, Faculty of Dentistry, Ataturk University, Erzurum
Source of Support: None, Conflict of Interest: None
| Abstract|| |
Purpose: To compare fracture resistance force (FRF) and failure types of crowns milled from resin nanoceramic (Lava Ultimate)-, and modified polymethylmethacrylate (PMMA) (Vita computer-aided design (CAD)-Temp)-, and PMMA (Telio CAD)-based CAD/computer-assisted manufactured (CAM) blocks. Materials and Methods: Three experimental groups of 10 milled crowns were arranged: Group-1 (Lava Ultimate), Group-2 (Vita CAD-Temp), and Group-3 (Telio CAD). Crowns were machined in sizes similar to a primary second molar stainless steel crown (SSC) and stored in water at 37°C for 30 days. The crowns were seated on Cr-Co dies. Their FRFs were measured using a universal test machine until fracture. FRFs and failure types were recorded and statistically analyzed (P < 0.05). Results: There were statistically significant differences among the groups for both FRFs and failure types. The sources of significant differences for FRFs and failure types were Group-3 and Group-1, respectively.
Conclusion: Crowns milled from different chemical structural CAD/CAM blocks may be used for restoration of primary molar teeth.
Keywords: Computer-aided design/computer-assisted manufactured resin, fracture resistance force, primary molar crowns
|How to cite this article:|
Mete A, Yilmaz Y, Derelioglu S S. Fracture resistance force of primary molar crowns milled from polymeric computer-aided design/computer-assisted manufactured resin blocks. Niger J Clin Pract 2018;21:525-30
|How to cite this URL:|
Mete A, Yilmaz Y, Derelioglu S S. Fracture resistance force of primary molar crowns milled from polymeric computer-aided design/computer-assisted manufactured resin blocks. Niger J Clin Pract [serial online] 2018 [cited 2020 Jan 25];21:525-30. Available from: http://www.njcponline.com/text.asp?2018/21/4/525/229083
| Introduction|| |
Stainless steel crowns (SSCs) were introduced by Dr Humphrey into the pediatric dentistry as an indirect restorative resolution in 1950. Over time, clinicians and manufacturers attempted to make some esthetic modifications such as open-faced SSC, chairside-veneered SSC, and preveneered SSC to provide esthetic solutions for their metallic gray-colored appearances.,, In common, the esthetic approaches comprise SSCs and esthetic resin material combinations. The combinations have raised not only some concerns in terms of both human health and environment but also have sometimes provided unsatisfactory resolutions for parents., Thus, researches have inclined the development of metal-free esthetic restorations. In the early 1980s, new- invented computer-aided design/computer-assisted manufacture (CAD-CAM) technology was introduced to produce metal-free esthetic restorations. Esthetic restorations are constructed with labside (dental lab-based, dental laboratory production-based, network or open-concept-based model) or chairside (in-office system model) CAD/CAM technologies and milled with alumina, zirconia, and porcelain-based ceramic blocks, metal alloy blocks, and various composite resin blocks. Chairside CAD/CAM technology is more advantageous than labside technology, since both restorations are prepared in a single appointment and also no temporary restorations are used.
Glass-ceramic material that is widely used with CAD/CAM technologies has both advantages such as the esthetic appearance, color stability, biocompatibility, and life-long durability and disadvantages such as brittleness, tendency to fracturing, and attrition on the enamel of the antagonist tooth.,,,, To overcome its disadvantages, resin nanoceramic (RNC)-, modified polymethylmethacrylate (PMMA)-, or PMMA-based polymeric resins have been developed under high temperature and pressure.,,, The polymeric materials have some advantages ,,,: they are less worn by the antagonist tooth enamel, their low modulus of elasticity enables them to absorb the functional stresses, they have a higher degree of conversion due to lower rate of residual monomer, and they require less invasive chamfer and bevel preparation types.
Although the studies have been conducted in relation to fracture resistance force (FRF) of crowns milled for permanent teeth, no results for primary molar crowns have been reported. The objective of this study was to compare occlusal FRFs and failure types of primary molar crowns milled from RNC-, modified PMMA-, and PMMA-based CAD/CAM blocks for in-office system model. The null hypothesis was that no significant difference would be found with regard to FRFs and failure types among primary molar crowns machined from the CAD/CAM blocks such as RNC-, modified PMMA-, and PMMA-based blocks.
| Materials and Methods|| |
Irreversible hydrocolloid impression material was placed in a plastic molds. #E2 (crown for primary second molar) SSCs (3M and ESPE, Seefeld, Germany) were immerged into the impression material up to 10 mm. The impression material was waited to be set. Inner surfaces of the SSCs in the impression material were sealed using Vaseline ® (Lever Faberge GmbH, 21614 Buxtehude, Germany). Both the inner surfaces of the SSCs and the entryway were filled with molten casting wax. After the wax pattern has set, it was removed from the dental impression material. Furthermore, the SSCs were delicately removed from the wax pattern. The preparations of the patterns were made as follows: occlusal surface was reduced by 1–1.5 mm and buccal, lingual, mesial, and distal surfaces were reduced by 15°–20° angle without any undercut remained. Gingival margin line was reduced by preparing a 0.5 mm bevel. Suitability of the wax pattern preparation was checked through the #E2 SSC on the wax pattern. Later, Cr-Co alloy metal dies were fabricated from the wax patterns. The cast dies were sandblasted using aluminum oxide particles. The cast abutment dies were embedded in acrylic resin up to 1 mm below the prepared gingival margin line and used for FRF test procedure of each crown.
Milling of the crowns from computer-aided design/computer-assisted manufactured blocks
The crown materials for the study are listed in [Table 1]. Lava Ultimate, Vita CAD-Temp, and Telio CAD CAD/CAM blocks were selected to mill the crowns.
|Table 1: Materials, compositions, and manufacturers as used in the study|
Click here to view
The crown designs were made in CEREC AC Acquisition Unit using CEREC 4.0 software (Sirona Dental Systems GmbH, Bensheim, Germany) since the program offers the use of biogeneric design technique (the software has data on all permanent tooth forms; however, it additionally scans the adjacent teeth to copy their characteristics). Permanent first molar forms were referenced due to their similarity to the forms of the primary second molars. Restoration type was selected as full crown. Biogeneric copy design was used as the biogeneric design technique [Figure 1]a, [Figure 1]b, [Figure 1]c.
|Figure 1: Choosing the tooth number for the upper (a) and lower (b) primary second molar crowns, restoration type, and biogeneric design method (c)|
Click here to view
CEREC MC XL (Sirona Dental Systems GmbH, Bensheim, Germany) was selected as the milling unit. The brand and type of the polymeric CAD/CAM resin block that would be used in the milling process were chosen and marked.
Optical impressions of the cast abutment dies were acquired by CEREC Omnicam (Sirona Dental Systems GmbH, Bensheim, Germany). Since biogeneric copy was used as the biogeneric design technique, to standardly simulate the morphologies of the teeth before the preparation, optical impressions of #E2 SSC were also acquired [Figure 2]a and [Figure 2]b. Crowns were designed based on this order.
|Figure 2: Screen shot scanned from the lower primary second molar cast abutment die (a); biogeneric copy of the lower #E2 stainless steel crown (b); conforming the margins of the crown (c); designing the lower primary second molar crown (d); virtual positioning scenario for the crown inside the Lava Ultimate block (e); virtual positioning scenarios for the crowns inside the Vita computer aided design-Temp and Telio computer-aided design blocks (f)|
Click here to view
After the optical impression process, models of the cast abutment dies and biogeneric copies of the SSCs were screened on the liquid-crystal display monitor. They were examined, and undesirable model areas were lined and cut out. Gingival margins of the restorations were manually plotted [Figure 2]c.
Acquired virtual models were dropped into the dental arcs in the standard image catalog of the software in accordance with their natural positions. Biogeneric copies are automatically obtained by the system [Figure 2]d.
For this in vitro study, since the impressions were taken over a single tooth, the proximal and occlusal contact force parameters determined by the system were eliminated. The parameters used for this study were minimal radial thickness = 1700 μm, minimal occlusal thickness = 1700 μm, and cement spacer = 80 μm. Crown design was made through the guidance of biogeneric copy [Figure 3].
Designed crowns are automatically dropped into as one crown for each Lava Ultimate CAD/CAM block [Figure 2]e and three crowns for each Vita CAD-Temp and Telio CAD blocks [Figure 2]f.
Soon after the restoration design had been completed, bur and block were placed in CEREC MC XL milling unit. By pushing the “start” button on the CEREC AC unit, milling process was begun in the CEREC MC XL milling unit. When the restoration was completely machined, the blocks were retrieved from the milling unit's chamber, and the restorations were cut out of the blocks. Specimens had been waited at 37°C for 30 days until the test period.
Group 1: Passive seatings of every crown that was milled out of Lava Ultimate blocks on the prepared Cr-Co cast-die were fit-tried. Each crown was cemented onto one of the cast abutment dies using temporary luting cement (Calcimol, Voco, Cuxhaven, Germany). The crown was held on the cast die under a constant force of 5 kg/f for 4 min.
Group 2: Every crown in the group was prepared by the milling of Vita CAD-Temp polymeric blocks, and passive seating on the cast abutment die was fit-tried. Next steps were conducted in the same methodology of Group-1.
Group 3: Passive seatings of the crowns milled from Telio CAD blocks were tried on the die-casted abutments. Crown cementation procedure was similar to those in Group-1.
Fracture resistance force test and failure types
#E2 (crown for primary second molar) SSC was immerged into the irreversible hydrocolloid impression material up to 10 mm. The SSC was removed from impression material after the impression material was set. The hollow was filled with molten casting wax. The wax pattern was removed from the impression material. Cr-Co alloy metal jig was fabricated and sandblasted using aluminum oxide particles. Using the fabricated Cr-Co loading jig, load tests were carried out. Load was applied on the occlusal surfaces of the crowns with a header rate of 1.5 mm/min (AGS-5kNG; Shimadzu Co., Kyoto, Japan) and the force required was recorded in newtons. Loading had continued until failures such as split-fracture (score 1), rupture, or plastic deformation (score 2) were detected on the crown materials and the obtained data were recorded in Newton. In addition, failures occurred were photographed under a stereomicroscope with ×10 magnification (Nikon SMZ-V multipoint-sensor system, Japan).
All analyses were carried out using SPSS 20.0 for Windows (SPSS, Chicago, IL, USA). The FRFs obtained from three materials were compared by using one-way analysis of variance and post hoc Duncan multiple comparison tests. Fracture types were compared using Chi-square test. The significance level was set at P < 0.05.
| Results|| |
The mean FRF values are given in [Table 2]. It is seen in the table that mean FRF values change from 866.8 to 898.1 newtons. One-way ANOVA revealed significant differences among the groups in terms of FRF test (F = 20.798 P<005). To understand the source of this significance, Duncan post hoc multiple comparison test was used. The distribution of FRFs occurred as follows: Group-3 > Group-1 = Group-2. That is, the mean FRF obtained from the crowns machined from Telio CAD was significantly higher than those of both Lava Ultimate and Vita CAD-Temp (P < 0.05).
|Table 2: The mean fracture resistance force values and failures types of the crowns|
Click here to view
The fracture types observed are showed in [Table 2] and [Figure 4]a, [Figure 4]b, [Figure 4]c, [Figure 4]d and [Figure 5]a, [Figure 5]b, [Figure 5]c, [Figure 5]d. When all three fracture types were compared, the difference among the groups found to be statistically significant (ċ2 = 8.459; P < 0.02). The source of the statistical difference was Group-1, and “fracture” failures (score 1) were noted in all of the crowns in this group [Figure 4]a and [Figure 4]b. Although there was no significant difference between Group-2 and Group-3, “plastic deformation” failures (score 2) in Group-3 were slightly higher than those of Group-2 [Figure 5]a, [Figure 5]b, [Figure 5]c, [Figure 5]d.
|Figure 4: Crowns displaying score 1 failure types; Lava Ultimate (a and b), Vita computer-aided design-Temp (c), and Telio computer-aided design (d) (×10)|
Click here to view
|Figure 5: Crowns demonstrating score 2 failure types; Lava Ultimate (a and b), Vita computer-aided design-Temp (c), and Telio computer-aided design (d) (×10)|
Click here to view
| Discussion|| |
Although in vitro studies are considered as a sign of clinical achievement, they might not completely prove the clinical expectancies since the clinical conditions could not be fully simulated. They provide the clinicians foreknowledge for deciding about the use of tested materials. From this point, the authors compared the FRFs of the crowns for the primary second molar, which were milled out of three different CAD/CAM resins. The differences between both the FRFs obtained from the groups and the fracture types were found statistically significant (P < 0.000). The null hypothesis stating, “there was no significant difference between the FRFs and failure types of primary molar crowns machined from the CAD/CAM blocks such as PMMA-, modified PMMA-, and RNC-based” has been rejected.
Morphological variations and irregularities of the natural tooth and the amount of the remaining dentin tissue after the preparation may influence the fracture resistance of the crowns. To eliminate the situation, artificial abutments with standardized preparation forms were used for this study. Stawarczyk et al. stated that in the FRF tests, fixed dental prosthesis might be tested by seating on the abutments without using cement. The moduli of elasticity of the abutments and cement have an influence on the fracture resistance of the restoration., As the modulus of elasticity of the abutment increases, the fracture resistance of the restoration raises. The cement may absorb the applied forces. Thus, the authors seated the PMMA-, modified PMMA-, and RNC-based CD/CAM crowns on the Cr-Co alloy abutments without adhesive.
PMMA synthetic polymers introduced in the 1930s are widely used in dentistry. These materials can be divided into the linear (e.g., PMMA) and the cross-linked polymers (e.g., Bis-GMA, TEGDMA, and UDMA). They have been used for crowns milled out of polymeric blocks in CAD/CAM technology as well as dentures, fillings and adhesive materials, and sealants.
Stawarczyk et al. found that Vita CAD-Temp specimens had lower FRFs than those of Telio-CAD. The result was in accordance with the present study. This may be explained by the organic structures of CAD/CAM blocks.,
Telio CAD is a high strength prefabricated monomethacrylate-based PMMA, and it has long-chain-shaped linear molecules, which are slightly cross-linked. Being an acrylate polymer, Vita CAD-Temp has vinyl groups in which 2 carbon atoms double bonded to one another and also attached to the carbonyl carbon. Since the double bonds are very reactive and display low strength, acrylates easily form polymers. Furthermore, H2O molecules diffuse the spaces among the polymer chains and make them apart. Yao et al. stated that water physically weakened Vita CAD-Temp more than Telio CAD.
Alt et al. found that the FRFs of the crowns milled from composite resin blocks containing UDMA, reduce as long as the crowns have been soaked in water. In this study, similar results were obtained from the crowns machined by using Lava Ultimate blocks because they were stored in water for 1 month before the testing. These findings may be attributed to hydrolytic degradation of the UDMA resin matrix of the Lava Ultimate. Polymers that contain urethane-based monomer system have hydrophilic tendency since their carbamate linkage may develop hydrogen bonds with water. Matsukawa et al. and Kerby et al. stated that using UDMA monomers could be an effective method for reducing the water sorption of urethane-based polymers.
The crowns milled from CAD/CAM blocks may show good clinical performance in primary molar teeth because they have resistance to fracture under the forces that were greater than the average biting force of 5–10-year-old children (375 newtons). The limitation of the study was that the loads were only axially applied. Parafunctional movements and lateral forces occurred in the mouth were not simulated.
Either deformation or fracture occurred on the crown material on which the load applied through the primary second molar shaped Cr-Co jig. If both surfaces (crown and jig) were rigid, fractures occurred on the crown material. Having been one of the surfaces, if the crown material had a ductile structure, it might absorb more functional stress through the plastic deformation., There were significant differences between the fracture types in this study [Table 2]. The authors consider that the filler ratio of the materials (Lava Ultimate 80% nanoceramic filler particles; Vita CAD-Temp 14% microparticle filler; Telio CAD no filler) and surface hardness (Lava Ultimate = 2.5 GPa; Telio CAD = 180 MPa; Vita CAD Temp = 210 MPa) may contribute to these differences. High resin ratio and low filler rate cause deformation on the material rather than the fracture. On the PMMA- and modified PMMA-based crowns, deformation may be observed instead of fracture. The fracture failures noted in all of the specimens may be explained by the higher surface hardness of the Lava Ultimate in comparison to the other materials used in the study.
| Conclusion|| |
Within the limitation of this study, CAD/CAM crowns milled for the primary molars promised to be used as an alternative for the full-coronal coverage. However, clinical studies are needed to support their use in the primary molar teeth restorations.
Financial support and sponsorship
This study has been conducted through the Ataturk University Scientific Research Projects Coordination Agency's support for the project no 2012/383.
Conflicts of interest
There are no conflicts of interest.
| References|| |
Humphrey WP. Uses of chrome steel in children's dentistry. Dent Surv 1950;26:945-9.
Roberts JF. The open-face stainless steel crown for primary molars. ASDC J Dent Child 1983;50:262-3.
Yilmaz Y, Koçoğullari ME. Clinical evaluation of two different methods of stainless steel esthetic crowns. J Dent Child (Chic) 2004;71:212-4.
Fuks AB, Ram D, Eidelman E. Clinical performance of esthetic posterior crowns in primary molars: A pilot study. Pediatr Dent 1999;21:445-8.
Yilmaz A, Ozdemir CE, Yilmaz Y. A delayed hypersensitivity reaction to a stainless steel crowns: A case report. J Clin Pediatr Dent 2012;36:235-8.
Carvalho AO, Bruzi G, Giannini M, Magne P. Fatigue resistance of CAD/CAM complete crowns with a simplified cementation process. J Prosthet Dent 2014;111:310-7.
Mormann WH. The original of the Cerec method: A personal review of the first 5 years. Int J Comput Dent 2004;7:11-24.
Strub JR, Rekow ED, Witkowski S. Computer-aided design and fabrication of dental restorations: Current systems and future possibilities. J Am Dent Assoc 2006;137:1289-96.
Hooshmand T, Parvizi S, Keshvad A. Effect of surface acid etching on the biaxial flexural strength of two hot-pressed glass ceramics. J Prosthodont 2008;17:415-9.
Jakob FM, Jungbauer G, Schneider J, Malyk Y, Edelhoff D, Hickel R, et al
. Biocompatibility of New CAD/CAM-Machinable Materials for Provisional Long-Term Restorations. Abstract 2280. Barcelona: IADR; 2010.
Stawarczyk B, Ender A, Trottmann A, Özcan M, Fischer J, Hämmerle CH, et al.
Load-bearing capacity of CAD/CAM milled polymeric three-unit fixed dental prostheses: Effect of aging regimens. Clin Oral Investig 2012;16:1669-77.
Krämer N, Kunzelmann KH, Taschner M, Mehl A, Garcia-Godoy F, Frankenberger R, et al.
Antagonist enamel wears more than ceramic inlays. J Dent Res 2006;85:1097-100.
Edelhoff D, Beuer F, Schweiger J, Brix O, Stimmelmayr M, Guth JF, et al.
CAD/CAM-generated high-density polymer restorations for the pretreatment of complex cases: A case report. Quintessence Int 2012;43:457-67.
Giordano R. Materials for chairside CAD/CAM-produced restorations. J Am Dent Assoc 2006;137 Suppl 1:14S-21S.
Tsitrou EA, Northeast SE, van Noort R. Evaluation of the marginal fit of three margin designs of resin composite crowns using CAD/CAM. J Dent 2007;35:68-73.
Lührs AK, Pongprueksa P, De Munck J, Geurtsen W, Van Meerbeek B. Curing mode affects bond strength of adhesively luted composite CAD/CAM restorations to dentin. Dent Mater 2014;30:281-91.
Keul C, Müller-Hahl M, Eichberger M, Liebermann A, Roos M, Edelhoff D, et al.
Impact of different adhesives on work of adhesion between CAD/CAM polymers and resin composite cements. J Dent 2014;42:1105-14.
Alt V, Hannig M, Wöstmann B, Balkenhol M. Fracture strength of temporary fixed partial dentures: CAD/CAM versus directly fabricated restorations. Dent Mater 2011;27:339-47.
Nguyen JF, Migonney V, Ruse ND, Sadoun M. Resin composite blocks via high-pressure high-temperature polymerization. Dent Mater 2012;28:529-34.
Johnson AC, Versluis A, Tantbirojn D, Ahuja S. Fracture strength of CAD/CAM composite and composite-ceramic occlusal veneers. J Prosthodont Res 2014;58:107-14.
Fischer H, Weber M, Eck M, Erdrich A, Marx R. Finite element and experimental analyses of polymer-based dental bridges reinforced by ceramic bars. J Biomech 2004;37:289-94.
Mahmood DJ, Linderoth EH, Vult Von Steyern P. The influence of support properties and complexity on fracture strength and fracture mode of all-ceramic fixed dental prostheses. Acta Odontol Scand 2011;69:229-37.
Scherrer SS, de Rijk WG. The fracture resistance of all-ceramic crowns on supporting structures with different elastic moduli. Int J Prosthodont 1993;6:462-7.
Vuorinen AM. Rigid Rod Polymer Fillers in Acrylic Denture and Dental Adhesive Resin Systems. Turun Yliopisto University of Turku; 2010. p. 10-1.
Yao J, Li J, Wang Y, Huang H. Comparison of the flexural strength and marginal accuracy of traditional and CAD/CAM interim materials before and after thermal cycling. J Prosthet Dent 2014;112:649-57.
Dyer SR, Lassila LV, Jokinen M, Vallittu PK. Effect of cross-sectional design on the modulus of elasticity and toughness of fiber-reinforced composite materials. J Prosthet Dent 2005;94:219-26.
Matsukawa S, Hayakawa T, Nemoto K. Development of high-toughness resin for dental applications. Dent Mater 1994;10:343-6.
Kerby RE, Tiba A, Knobloch LA, Schricker SR, Tiba O. Fracture toughness of modified dental resin systems. J Oral Rehabil 2003;30:780-4.
Bakke M, Holm B, Jensen BL, Michler L, Möller E. Unilateral, isometric bite force in 8-68-year-old women and men related to occlusal factors. Scand J Dent Res 1990;98:149-58.
Magne P, Perakis N, Belser UC, Krejci I. Stress distribution of inlay-anchored adhesive fixed partial dentures: A finite element analysis of the influence of restorative materials and abutment preparation design. J Prosthet Dent 2002;87:516-27.
Stawarczyk B, Özcan M, Trottmann A, Schmutz F, Roos M, Hämmerle C, et al.
Two-body wear rate of CAD/CAM resin blocks and their enamel antagonists. J Prosthet Dent 2013;109:325-32.
Drummond JL. Degradation, fatigue, and failure of resin dental composite materials. J Dent Res 2008;87:710-9.
[Figure 1], [Figure 2], [Figure 3], [Figure 4], [Figure 5]
[Table 1], [Table 2]